Tb<sub>2-x</sub>Nd<sub>x</sub>Zn<sub>17-y</sub>Ni<sub>y</sub> (x = 0.5, y = 4.83): a new intermetallic with a maximum disordered structure and its hydrogen storage properties.
Nytka, Vitalii; Kordan, Vasyl; Stetskiv, Andrij; Pavlyuk, Volodymyr; Acta crystallographica. Section C, Structural chemistry 79 (2023) 257–262; doi:10.1107/S2053229623004369

data_2312111
_publ_section_title
;
 Tb<sub>2-x</sub>Nd<sub>x</sub>Zn<sub>17-y</sub>Ni<sub>y</sub> (x&#xa0;=
 0.5, y&#xa0;= 4.83): a new intermetallic with a maximum disordered
 structure and its hydrogen storage properties.
;
_journal_coeditor_code           YP3229
_journal_issue                   'Pt 6'
_journal_name_full
'Acta crystallographica. Section C, Structural chemistry'
_journal_page_first              257
_journal_page_last               262
_journal_paper_doi               10.1107/S2053229623004369
_journal_volume                  79
_journal_year                    2023
_chemical_formula_iupac          'Tb1.51 Nd0.51 Zn12.17 Ni4.83'
_chemical_formula_sum            'Nd0.51 Ni4.83 Tb1.51 Zn12.17'
_chemical_formula_weight         1389.69
_space_group_crystal_system      trigonal
_space_group_IT_number           166
_space_group_name_Hall           '-R 3 2"'
_space_group_name_H-M_alt        'R -3 m :H'
_audit_creation_method           SHELXL-2014/7
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            3
_cell_length_a                   9.0637(5)
_cell_length_b                   9.0637(5)
_cell_length_c                   13.2319(10)
_cell_measurement_reflns_used    2378
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      27.436
_cell_measurement_theta_min      3.017
_cell_volume                     941.38(10)
_computing_cell_refinement
;
CrysAlis CCD (Oxford Diffraction, 2008)
;
_computing_data_collection
;
CrysAlis CCD (Oxford Diffraction, 2008)
;
_computing_data_reduction
;
CrysAlis RED (Oxford Diffraction, 2008)
;
_computing_molecular_graphics
;
DIAMOND (Brandenburg, 2006)
;
_computing_publication_material
;
SHELXL2014 (Sheldrick, 2015b) and
publCIF (Westrip, 2010)
;
_computing_structure_refinement
;
SHELXL2014 (Sheldrick, 2015b)
;
_computing_structure_solution
;
SHELXS2014 (Sheldrick, 2015a)
;
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.983
_diffrn_measured_fraction_theta_max 0.986
_diffrn_measurement_device_type  'Oxford Diffraction Xcalibur3 CCD'
_diffrn_measurement_method       '\w scans'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.1616
_diffrn_reflns_av_unetI/netI     0.1036
_diffrn_reflns_limit_h_max       11
_diffrn_reflns_limit_h_min       -11
_diffrn_reflns_limit_k_max       11
_diffrn_reflns_limit_k_min       -11
_diffrn_reflns_limit_l_max       17
_diffrn_reflns_limit_l_min       -17
_diffrn_reflns_number            2378
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         27.436
_diffrn_reflns_theta_min         3.017
_diffrn_source                   'fine-focus sealed tube'
_exptl_absorpt_coefficient_mu    40.109
_exptl_absorpt_correction_T_max  0.782
_exptl_absorpt_correction_T_min  0.563
_exptl_absorpt_correction_type   analytical
_exptl_absorpt_process_details
;
(CrysAlis RED; Oxford Diffraction, 2008)
;
_exptl_crystal_colour            'metallic dark grey'
_exptl_crystal_density_diffrn    7.354
_exptl_crystal_density_meas      7.34(3)
_exptl_crystal_density_method    volumetric
_exptl_crystal_description       plate
_exptl_crystal_F_000             1884
_exptl_crystal_size_max          0.06
_exptl_crystal_size_mid          0.04
_exptl_crystal_size_min          0.01
_refine_diff_density_max         2.227
_refine_diff_density_min         -2.037
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   0.900
_refine_ls_matrix_type           full
_refine_ls_number_parameters     22
_refine_ls_number_reflns         285
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      0.900
_refine_ls_R_factor_all          0.0861
_refine_ls_R_factor_gt           0.0460
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.0421P)^2^] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0866
_refine_ls_wR_factor_ref         0.0960
_reflns_number_gt                176
_reflns_number_total             285
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            yp3229sup1.cif
_cod_data_source_block           I
_cod_depositor_comments          'Adding full bibliography for 2312111.cif.'
_cod_original_cell_volume        941.38(13)
_cod_database_code               2312111
_cod_database_fobs_code          2312111
_shelx_hkl_checksum              90776
_shelx_res_checksum              7684